w IN SUPPLEMENT TO THE WELDING JOURNAL, NOVEMBER 1973
Sponsored by the American Welding Society and the Welding Research Council m
A Quantitative Weldability Test for Susceptibility to Lamellar Tearing
Su/tab/e for laboratory use, the test shows AI-Si killed steels to be less susceptible than Si killed steels
BY R. P. OATES A N D R. D. STOUT
ABSTRACT. An important aspect of current research on lamellar tearing is the development of a testing tech-nique that wi l l provide a quantitative assessment of material susceptibility. The majority of investigations have approached this problem in an indi-rect manner, attempting to correlate short transverse material properties to lamellar tearing susceptibility. This approach requires that the lamellar tearing resistance of the material already be known. Weldabil i ty tests are the most realistic technique for directly evaluating lamellar tearing susceptibility but they have been l im-ited in the past by the cost of testing and the difficulties in quantifying and in interpreting the results. This report describes the development and eval-uation of a quantitative weldabil i ty test (the Lehigh lamellar tearing test) to overcome these limitations.
Lamellar tears were generated wi th the Lehigh lamellar tearing test specimen in three of four materials in-vestigated. These materials repre-sented a wide range of lamellar tear-ing susceptibility. The test made it possible to measure a quantitative ex-ternal restraint level required to pro-duce a critical size lamellar tear. The magnitude of this external restraint
R. P. OATES is associated with Wright Air Force Materials Laboratory and R. D. STOUT is Dean of the Graduate School, Lehigh University, Bethlehem, Pa.
level proved to be consistent w i th in-formation on the lamellar tearing sus-ceptibility obtained from actual shop fabrication experience. The restraint required to cause lamellar tearing was correlated w i th selected aspects of the short transverse mechanical properties and the inclusion distr ibu-tion in the material. The Lehigh test results were closely reproducible for the steels sensitive to lamellar tear-ing but were less consistent for a mar-ginal steel for wh ich loads wel l above the yield strength of the material were necessary to cause failure.
Wi th the Lehigh test results as a measure of lamellar tearing suscep-tibility, the relationship between in-clusion content and distribution, short transverse mechanical prop-erties and lamellar tearing suscep-tibil ity were investigated. The results showed a clear correlation between the tension test elongation, the room temperature Charpy test energy and the lamellar tearing susceptibility only if these short transverse test values were obtained in the region of potential tearing, generally w i th in % inch distance from the weld. Predic-tions of tearing susceptibility are often unreliable when they are de-rived from the short transverse prop-erties of regions at a greater depth in the plate thickness. Reduction in area measurements did not correlate very consistently w i th lamellar tearing susceptibility.
The results of this investigation also revealed differences in the mech-anism of lamellar tearing in the Si killed steel versus the Al-Si killed steels. These differences were attrib-uted to differences in inclusion type and to the britt le fracture transit ion temperature. The tests demonstrated that the lamellar tearing resistance of the Si killed steel could be improved 35% by preheating to above the brittle fracture transition temperature.
In t roduct ion
Lamellar tearing is a form of crack-ing that occurs in the base metal of weldments due to the combined effects of the anisotropic charac-teristics of hot rolled steel plate and high stresses generated by weld ther-mal contraction acting perpendicular to the rolling plane. This cracking is usually associated wi th highly re-strained Tee or corner joints where the weld fusion boundary is parallel to the rolling plane of the plate. The metallographic profile of a lamellar tear is characterized by terrace frac-ture surfaces parallel to the rolling plane of the plate joined in a step-like manner by shear wal l fractures per-pendicular to the rolling plane. The terrace fracture surfaces are shown to be associated wi th elongated or aligned inclusions, a material charac-teristic which also causes poor short transverse mechanical properties.
Lamellar tearing is not a new phe-
W E L D I N G R E S E A R C H S U P P L E M E N T ! 481-s
nomenon. It has undoubtedly existed since the inception of fusion welding on large wrought steel structures. It was not until the demand for high integrity structures necessitated the use of more sophisticated nondestruc-tive testing procedures that lamellar tears were identified. Today lamellar tearing is reported to be a problem in shipbuilding, atomic power plant con-s t ruc t i on , br idge c o n s t r u c t i o n , building construction, boiler fabrica-tion and in the construction of chem-ical and nuclear pressure vessels, offshore dri l l ing rigs and rail cars. The steel manufacturers and fabrica-tors are concerned about lamellar tearing for reasons such as the fo l -lowing:
Fig. 1 The fixture and welding facility for the Lehigh lamellar tearing test
1 The tearing can destroy the integ-rity of the joint.
2. Unless ultrasonic examination is carried out, lamellar tears are very difficult to detect and may go unde-tected until a service failure occurs.
3. The repair procedures for lamellar tearing are difficult, costly, usually t ime consuming and occasionally impracticable.
4. There is currently no generally acceptable procedure for assess-ing material susceptibility to lamel-lar tearing.
The development of a quantitative test for accurately measuring lam-ellar tearing susceptibility is there-fore an important aspect of current lamellar tearing research.
Investigators have addressed this problem indirectly by comparing the service history of the plate w i th such parameters as the short transverse mechanical properties, the ultrasonic attenuation properties or the inclu-sion content and distribution of the plate. The effectiveness of these parameters as useful quantitative measures of lamellar tearing suscep-tibility is l imited experimentally by the lack of a direct quantitative meas-ure of lamellar tearing susceptibility to verify these indirect correlations and conceptually by their failure to simulate testing conditions common to lamellar tearing service applica-tions.
Weldabil ity testing as a direct measure of lamellar tearing suscep-tibility is appealing because this type of testing may be designed to closely simulate actual service conditions. The effects of welding variables, ma-terial variables and restraint vari-ables can all be studied w i th this type of testing. Several researchers have
4 5 '
Fig. 2 Arrangement of the test specimen and cantilever beam for obtaining quantita-tive restraint
been successful in creating lamellar tears in the research laboratory (Refs. 8, 1 1 , 23, 26). Unfortunately the quantitative measures of lamellar tearing susceptibility have been dif f i -cult to interpret and reproduce and the testing procedures have been ex-pensive.
The purpose of this paper is to de-scribe the development and effective use of a new lamellar tearing we ld-ability test for quantitatively meas-uring susceptibil i ty to l ame l la r tearing.
Exper imenta l Procedure
Development of Weldability Test Procedure
The design criteria for a quantita-tive lamellar tearing weldabil i ty test are defined by production require-ments. These criteria include the fol lowing: 1 The test must be versatile enough
to produce lamellar tearing over a range of materials, welding condi-tions, and restraint severity.
2.The test results must be easy to interpret.
3. The test results must be repro-ducible w i th in the limits estab-lished by variations in the charac-teristics of the steel.
4. The test must be economical to perform and analyze. Lamellar tearing may occur under
two conditions of loading. The f irst (called rotation type lamellar tearing in this paper) occurs when the mem-bers being welded are free to rotate. The Cranfield specimen produces rotation-type lamellar tearing. The second type of lamellar tearing (called pull-type lamellar tearing in this paper) occurs when the members being welded are restrained from rotating. Crack initiation usually occurs below the plate surface and is seldom associated wi th the root of the weld. Numerous attempts have been made to produce pull-type tears in laboratory size specimens econom-ically. The results show that massive structural restraint is required if ade-quate short transverse plastic strains are to be produced by weld contrac-tion alone. Since this restraint is troublesome to create and difficult to analyze quantitatively, a more con-venient means of generating short transverse strain (to be used to sup-plement weld thermal strain) was sought. The Lehigh lamellar tearing test uses an external load applied during welding for this purpose.
A welding fixture (Fig. 1) was con-structed to permit the deposition of a single-bevel groove weld between the test specimen and a cantilever beam under variable degrees of exter-nal restraint provided by external hy-draulic loading. The setup is schemat-
482-s I N O V E M B E R 1 9 7 3